Eﬀect of Alumina Content on the Mechanical Properties
of Alumina Particle Dispersion Magnesium
, Kiyoshi Kuroda1
, Yukio Kasuga1
, Masahiro Yokouchi2
and Kei Ameyama4
1Department of Intelligent Mechanical Systems, College of Engineering, Tamagawa University, Tokyo 194-8610, Japan
2Kanagawa Industrial Technology Center, Ebina 243-0435, Japan
3Ritsumeikan Global Innovation Research Organization, Ritsumeikan University, Kusatsu 525-8577, Japan
4Department of Mechanical Engineering, College of Science and Engineering, Ritsumeikan University, Kusatsu 525-8577, Japan
To enhance the mechanical properties of magnesium (Mg) alloys, powders of pure Mg (Al2O3/Mg) dispersed with over 10 vol% alumina
(Al2O3) particles were made by ball milling powder mixtures of pure Mg and Al2O3particles with particle sizes of 0.3 and 1mm. The eﬀect of
the Al2O3content of hot-pressed discs formed from the Al2O3/Mg powders on the mechanical properties of the discs was investigated. The
Al2O3particles were found to be uniformly dispersed in the Al2O3/Mg discs. The hardness of the discs increased sharply at an Al2O3content of
20 vol%. This is considered to be because of the excellent interfacial bonding between Mg and Al2O3when the Al2O3/Mg discs contain a
suﬃcient amount of Al2O3particles and have a suﬃcient interparticle distance. The maximum hardness of a 20 vol% Al2O3/Mg disc (with an
Al2O3particle size of 0.3mm) was 220 HV, which is much higher than the hardness of AZ91 Mg alloys. The bending strength of the Al2O3/Mg
discs increased from 0 to 10 vol% Al2O3and then decreased from 20 vol% Al2O3. It is considered that the 0 and 10 vol% discs have similar
fracture deﬂections and that the 10 vol% discs with Al2O3particles can withstand higher compression and tension forces than the 0 vol% discs
which do not contain any particles. The reason for the lower bending strength of the 20 vol% Al2O3disc is thought to be because it is harder and
more brittle, making it easier for voids to form in the discs, and thus making it easier for cracks to propagate on the specimen surface. [doi:10.2320/matertrans.M2010060]
(Received February 18, 2010; Accepted July 9, 2010; Published August 25, 2010)
Keywords: alumina particle dispersion magnesium powder, attritor ball mill, hot pressing, microstructures, hardness, bending strength
In recent years, advances in automotive lighting have led to an increase in the demand for magnesium (Mg) alloys, which are lightweight substitutes for aluminum (Al) alloys. However, Mg alloys generally have inferior mechanical properties to Al alloys.
One potential method to improve the mechanical pro-perties of Mg alloys is to form composites of Mg alloys and ceramic particles and/or ﬁbers. Recently, composites of pure Mg or Mg alloys with ceramic particles and/or ﬁbers have been fabricated by casting and powder metal-lurgical processes. These composites have been widely studied.
The fabrication of composites of pure Mg reinforced by
alumina (Al2O3) particles by the powder metallurgical
process has been studied.1–4) In an attempt to improve the
dispersion strengthening of Mg in Al2O3, instead of mixing
pure Mg powder with several vol% of Al2O3 nanoparticles,
Unverrichtet al.4)ball milled the two powders to uniformly
disperse Al2O3 particles in Mg. When investigating the
dispersion strengthening, an Al2O3 content of several vol%
However, little research has been conducted on uniform
dispersions of over 10 vol% Al2O3 particles in pure Mg
powder produced by mechanical milling pure Mg and Al2O3
particles. The hardness and the wear resistance of a powder of over 10 vol% Al2O3particles uniformly dispersed in pure Mg
(Al2O3/Mg) are expected to be higher than those of an Al2O3
dispersion strengthened powder, because the strength of Al2O3particles will enhance that of the Al2O3/Mg powder.
The surface properties of pure Mg or Mg alloys are
expected to be improved by bonding Al2O3/Mg to Mg
substrates using processes such as plasma spraying or hot rolling.5)
Moreover, Al2O3/Mg powders can be used to fabricate
sintered compacts that have superior mechanical properties by various pressure sintering processes such as hot pressing, hot isostatic pressing, spark plasma sintering and hot roll sintering.6)
We have made Al2O3/Mg powders by ball milling powder
mixtures of pure Mg powder and 0–22.7 vol% Al2O3
particles with Al2O3 particle sizes of 1mm. We then
investigated the mechanical properties of hot-pressed discs obtained from these Al2O3/Mg powders and found that they
have higher hardnesses than AZ91 Mg alloys.7)
In the present study, the eﬀect of the Al2O3content of the
hot-pressed discs fabricated from over 10 vol% Al2O3/Mg
powders with Al2O3 particle sizes of 0.3 and 1mmon the
mechanical properties of the discs was investigated.
2. Experimental Procedures
2.1 Test powders
Pure magnesium powder with a particle size of 180mm,
(Mg powder, Kojundo Chemical Laboratory Co. Ltd.; purity: 99.5%) and-alumina particles with particle sizes of 0.3 and
1mm (Al2O3 particles, Kojundo Chemical Laboratory Co.
Ltd.; purities: 99.99% and 99.9%, respectively) were used as the starting materials.
2.2 Trial process
Figure 1 depicts the trial process for Al2O3 particle
ders were milled in an attritor ball mill. Powder mixtures of 200 cm3Mg and 0–30 vol% Al2O3particles were fed into an
Al2O3 container together with 3 dm3 5 mm diameter Al2O3
balls. Mixtures of Al2O3 particles with Mg powder with
Al2O3 particle contents of 0, 10, 20, and 30 vol% were
The Al2O3agitator arm was rotated at 300 rpm for 180 ks
in an argon atmosphere to mill the mixed powders. 2 mass% stearic acid was added as a lubricant. The obtained Al2O3/
Mg powders were compacted into green discs using a hydraulic press at 637 MPa for 60 s. The green discs were hot compressed at 40 MPa and 848 K for 3.6 ks in a carbon sample holder with an argon atmosphere. The furnace was
then cooled to room temperature and Al2O3/Mg discs were
The average particle sizes of the Al2O3/Mg powders were
obtained by measuring the size distribution using a laser diﬀraction particle size analyzer (Sympatec GmbH, Helos & Lodos). Al2O3/Mg discs with a disc thickness tolerance of
0:05mm were ﬁnished by polishing with abrasive paper
and buﬃng. Microstructural observations and qualitative analysis of the Al2O3/Mg powders and discs were performed
using an optical microscope (Olympus Co. Ltd., STM5-UM), a ﬁeld-emission scanning electron microscope (SEM; Hitachi Ltd., S-4300SE), an electron probe microanalyzer (EPMA, Jeol Ltd., JXA-8500F), and an x-ray diﬀractometer (Philips Co. Ltd., X’pert Pro MPD).
The disc densities were measured using a hydrometer. The relative density was obtained by dividing the measured density by the theoretical density:
whereRis the relative density,is the measured density of
a disc, and 0 is the theoretical density (e.g., Mg-10 vol%
Al2O3has a theoretical density of1:96103kg/m3).
The hardness of the Al2O3/Mg discs were measured using
a Vickers hardness tester at 49 N for 10 s. Five values were measured for each of the three discs.
The Al2O3/Mg discs were machined to give plates with
dimensions of 19.6 mm (length) 5 mm (width) 1.4 mm
(thickness). After buﬃng both surfaces, the plates were used in bending tests. The bending strength was calculated using the following formula for a beam:
whereFis the bending strength,Pmaxis the maximum load,
L is the distance between the support points, d is the
specimen width, andtis the specimen thickness. Values were obtained for ﬁve to six discs. All discs failed at the center of span.
3. Results and Discussion
3.1 Observations of Al2O3/Mg powders and discs
3.1.1 Al2O3/Mg powders
Figure 2(a) and (b) respectively show SEM images of the
surface and the cross-section of the 20 vol% Al2O3/Mg
powder with an Al2O3 particle size of 1mm. Figure 2(a)
shows the size variation of the Al2O3/Mg powder. The
average powder size was about 20mm. The other powders
exhibited similar morphologies and average sizes.
The recovery ratio of Al2O3/Mg powder extracted from
the ball-mill decreased because the volume of powder
solidiﬁcation by milling increases with increasing Al2O3
The average particle size of Al2O3/Mg powders is
considered to remain approximately constant with increasing
Al2O3 content, because although the Al2O3/Mg powders
become ﬁner with increasing Al2O3 content, they are more
likely to agglutinate at higer Al2O3contents.
Figure 2(c) is a high magniﬁcation image of Fig. 2(b). Elemental analysis for Mg, Al, and O using EPMA revealed that the gray regions in Fig. 2(c) are Mg and the ﬁne white particles are Al2O3 particles. Figures 2(b) and (c) show that
the Al2O3 particles are uniformly dispersed in the Mg
powder. Similar tendencies were observed for the other Al2O3/Mg powders.
3.1.2 Al2O3/Mg discs
Figure 3(a) shows a photograph of an Al2O3/Mg disc and
Fig. 3(b)–(g) show SEM images of 10, 20, 30 vol% Al2O3/
Mg discs. Figure 3(b), (d), and (f) show discs made from the 1mmAl2O3 particles and Fig. 3(c), (e), and (g) show discs
made from the 0.3mmAl2O3particles.
The discs had diameters in the range 20–21 mm and
thicknesses in the range 1.5–2.0 mm. Al2O3 particles are
uniformly dispersed in the Mg in all the discs; voids are present in the 30 vol% discs.
Figure 4 shows the Al2O3 particle amount per 100mm2
and the interparticle distance as functions of Al2O3content;
these values were measured from the SEM images in
Fig. 3(b)–(g) and other SEM images. The Al2O3 particle
amount increased and the interparticle distance decreased with increasing Al2O3 content. The 0.3mm Al2O3 particles
have a higher particle density and a smaller interparticle distance than the 1.0mmAl2O3 particles.
The measured Al2O3 particle amount is much higher than
the calculated particle densities. For all Al2O3 contents, the
Al2O3 particle sizes determined from the measured Al2O3
particle amount was about 0.2 and 0.3mmfor particle sizes of
0.3 and 1.0mm, respectively. These measured values are
almost the same as the median size of 100 Al2O3particles in
SEM images. The particles sizes used in this study (0.3 and Hot pressing
637MPa × 60s Cold pressing Pure Mg powder
Ar, 300rpm × 180ks
T=848K, 40MPa × 3.6ks Stearic acid (d= 180 µm)
(0 - 30vol%) (d= 0.3, 1µm)
10K / min Attritor ball mill
Hydraulic press Al2O3 particle
(Al2O3 / Mg) discs
1.0mm) represent the median sizes obtained by measuring size distributions by laser diﬀractometry. Even although diﬀerent methods were used to measure the particle size, the Al2O3 particles in the Al2O3/Mg powders and discs are
considered to have become ﬁner than the original Al2O3
3.2 Properties of Al2O3/Mg discs
Figure 5 shows the eﬀect of Al2O3content on the relative
density of the Al2O3/Mg discs. The relative density of the 0–
20 vol% Al2O3/Mg discs exceeds 100%. This is assumed to
be due to the formation of MgO by oxidation of the Mg powder as a result of exposure to air when ball milling the
Al2O3/Mg powders with active surfaces and of vaporization
of stearic acid when heating the green compacts. Addition-ally, the solid-state reaction of Mg and Al2O3particles is also
considered to have an eﬀect.
SEM observations of the 0–20 vol% discs reveal that the discs do not contain signiﬁcant amounts of microscopic pores. The discs are thus considered to have been fully densiﬁed.
The relative density of the 30 vol% discs is less than 100%. This is assumed to be due to their lower sinterabilities because of their lower workabilities as a result of their higher Al2O3contents.
Figure 6 shows the eﬀect of Al2O3content on the Vickers
hardness of the Al2O3/Mg discs. The Vickers hardness of
AZ91 alloys are also shown for comparison (these values were obtained by converting from the Brinell hardness numbers given in Ref. 8)).
For both Al2O3 particle sizes, the hardness of the Al2O3/
Mg discs decreased slightly when the Al2O3content
increas-ed from 0 to 10 vol%, increasincreas-ed sharply at 20 vol%, and decreased at 30 vol%. The discs containing the 0.3mmAl2O3
particles had higher hardness than those containing the
1.0mm Al2O3 particles. The maximum hardness of the
20 vol% Al2O3/Mg discs is 220 HV, which is much higher
than those of the AZ91 Mg alloys (indicated by the diagonal line in Fig. 6).
The following possible causes for the sharp increase in the
hardness in the 20 vol% Al2O3/Mg discs are discussed
(1) Al2O3particle dispersion strengthening
(2) Inhibition of Mg grain growth
(3) Solid-state reaction of Mg with Al2O3particles
(4) Interfacial bonding between Mg and Al2O3particles
(1) Al2O3particle dispersion strengthening
To consider the eﬀect of Al2O3 particle dispersion
strengthening, the stress necessary to pass dislocations between dispersed particles (known as ‘‘Orowan stress’’) was investigated.
The Orowan stressois given by:
whereTis line tension of dislocation,llis the average Al2O3
particle spacing, andbis Burgers vector.
T=b is assumed to be constant. The ratio of the Orowan
stress of the 20 and 10 vol% Al2O3/Mg discs were obtained
from the average Al2O3particle spacing for particle sizes of
0.3 and 1mm (see Fig. 4). The ratios were 1.1 and 1.4 for
Al2O3 particle sizes of 0.3 and 1mm, respectively. The
Orowan stress increaseed little with increasing Al2O3
In contrast, the ratio of the Vickers hardnesses of discs with Al2O3 contents of 20 and 10 vol% are 3.6 and 3.0 for
Al2O3particle sizes of 0.3 and 1mm; these ratios are greater
than the Orowan stress ratio.
Therefore, Al2O3 particle dispersion strengthening is
considered to have very little eﬀect because there almost no correlation between the Vickers hardness and the Orowan stress.
(2) Inhibition of Mg grain growth
Mg grain growth is considered to be inhibited with
increasing Al2O3 particle content during hot pressing.
Figure 7 shows optical microstructures of the 10 vol% and 20 vol% discs. The discs were electrolytically etched and the Mg grain sizes were measured. All the discs have Mg grain
sizes in the range 5–8mm. The 0 and 30 vol% discs have
similar grain sizes.
Al2O3particles are considered to be present in both the Mg
grains and grain boundaries, because the Al2O3interparticle
distance is 0.15–0.3mm(see Fig. 4), and the Al2O3particles
are uniformly dispersed in Mg (Fig. 3(b)–(g)).
Fig. 3 (a) Appearance of Al2O3/Mg disc. SEM images of 10 vol% Al2O3/Mg discs with Al2O3particle sizes of (b) 1mmand (c) 0.3mm,
20 vol% Al2O3/Mg discs with Al2O3particle sizes of (d) 1mmand (e) 0.3mmand 30 vol% Al2O3/Mg discs with Al2O3particle sizes of
There is considered to be very little inhibition of Mg grain growth with increasing Al2O3particle density, because grain
growth is independent of the Al2O3 particle size and the
(3) Solid-state reaction of Mg with Al2O3particles
The compound produced by the solid-state reaction of Mg with Al2O3particle is considered to increase with increasing
amount of Al2O3particles. Figure 8 shows X-ray diﬀraction
(XRD) results for Al2O3/Mg discs with diﬀerent Al2O3
contents. As shown in Fig. 8, magnesium oxide (MgO) is identiﬁed in all the discs, in addition to Mg and Al2O3. An
XRD peak assigned to an Al–Mg intermetallic compound (Mg17Al12) is detected for the 20 vol% disc with an Al2O3
particle size of 0.3mmand for the 30 vol% discs, in addition to peaks due to Mg, Al2O3, and MgO.
Moreover, although MgAl2O4 is considered to be
pro-duced by the solid-state reaction of MgO and Al2O3,9) it
could not be identiﬁed in the XRD results of the present study.
Figure 9 shows X-ray relative intensities for Mg (101) and MgO (220) of the Al2O3/Mg discs indicated by the arrows in
Fig. 8. The relative intensity of the Al2O3/Mg discs increases
with increasing Al2O3 content. The amount of MgO is
considered to increase due to the solid-state reaction of Mg with Al2O3 particles progressing with increasing Al2O3
The solid-state reaction of Mg with Al2O3 particles is as
Al is considered to be soluble in Mg due to the production
of MgO by the reaction. Equation (4) shows that Mg17Al12
is produced when the Mg solid solution exceeds the solid solubility limit of Al to Mg.
For the 20 vol% discs, Mg17Al12is detected only from the
disc with an Al2O3 particle size of 0.3mm. This is thought
0 200 600
10 20 30
Al2O3 Content (vol%)
400 800 1000
0.1 0.2 0.3 0.4
Al2O3 particle size
d = 0.3µm (Measured)
d = 1µm (Mea.)
d = 1µm
d = 0.3µm d = 0.3µm (Calculated)
d = 1µm (Cal.)
Fig. 4 Al2O3 particle amount and interparticle distance as functions of
Al2O3content in Al2O3/Mg discs.
80 90 100 110
10 20 30 0
Relative Density (%)
Mg (testing powder)
Al2O3 particle size
Fig. 5 Eﬀect of Al2O3 content on the relative density of the Al2O3/Mg
150 200 250
Mg (testing powder) AZ918)
Fig. 6 Eﬀect of Al2O3content on the Vickers hardness of the Al2O3/Mg
to be because the ﬁner Al2O3 particles react more readily
with Mg due to their larger contact area with the Al2O3
The precipitation hardening of Mg17Al12is thought to have
little eﬀect on the sharp increase in the hardness of the discs, because the XRD results reveal that only a small amount of
Mg17Al12 is produced and because the deference of the
hardness between pure Mg and precipitation-hardened AZ91 Mg alloy is not so great (the pure Mg (sand casting) and the
AZ91 Mg alloy (sand casting and T6 temper) are 30HB10)and
70HB,8)respectively). Moreover, both the MgO products and
solid solution hardening of Mg with Al are thought to have little eﬀect on the hardness since the 10 vol% discs have a similar hardness to the 0 vol% discs.
(4) Interfacial bonding between Mg and Al2O3 particles
To investigate the interfacial bonding between Mg and Al2O3 particles, we observed indentations produced by the
Vickers hardness test. Figure 10 shows the results. The edge of the plastically deformed indentation reveals that no abrasion occurs at the interface between the Mg and Al2O3
particles. Based on the results, the sharp increase in the hardness observed at 20 vol% is considered to be due to
excellent interfacial bonding between Mg and Al2O3
par-ticles, because terms of (1)–(3) are considered to have very little eﬀect on the sharp increase.
Therefore, the sharp increase in the hardness is predicted to promote Al2O3 particle strengthening because of the
hard-ness of the Al2O3 particles and the restraining eﬀect of the
Fig. 7 Optical microstructures of 10 vol% Al2O3/Mg discs with Al2O3particle sizes of (a) 1mmand (b) 0.3mmand 20 vol% Al2O3/Mg
discs with Al2O3particle sizes of (c) 1mmand (d) 0.3mm.
20° 30° 40° 50° 60° 70° 80° 90°
Cu K α MgO
30 vol% Mg (101)
Diffraction Angle, 2 θ
20° 30 40° 50° 60° 70° 80° 90°
Diffraction Angle, 2 θ
Cu K α
20 vol% 30 vol% 0 vol%Al2O3
Mg matrix as a result of the excellent interfacial bonding
between Mg and Al2O3 particles. This will occur when the
Al2O3/Mg discs contain a suﬃcient amount of Al2O3
particles with a suﬃcient interparticle distance.
The solid-state reaction of Mg with Al2O3 particles may
contribute to the excellent interfacial bonding. However, detailed observations and analysis by transmission electron microscopy are necessary to conﬁrm this conjecture.
3.2.3 Bending strength
Figure 11 shows the eﬀect of Al2O3 content on the
bending strength of Al2O3/Mg plates. For both Al2O3
particle sizes, the 10 vol% plates have a higher bending strength than the 0 vol% plates. It is considered that both plates have similar fracture deﬂections, and that the 10 vol%
plates containing Al2O3 particles can withstand higher
compression and tension forces than the 0 vol% plate which
does not contain any particles. The 20 vol% plates have lower bending strengths than the 10 vol% plates. This is thought to be because the plate becomes harder and more brittle, making it easier for voids to form in the discs. Based on these results, it considered that cracks generated on the specimen surface propagate more easily. This is supported by the observation of voids in the 30 vol% discs (see Fig. 3(f) and (g)) and indentation cracks were not observed after the Vickers hardness test for the 0 and 10 vol% discs, whereas they were observed for the 20 and 30 vol% discs.
The discs containing 0.3mmAl2O3 particles have higher
bending strengths than those containing 1.0mm Al2O3
Nobre et al.11) have reported that AZ31 wrought
magne-sium alloys have a four-point bending strength of 200– 220 MPa for a compressive strain of 2.5%. Although it is
Fig. 10 (a) Image of Vickers hardness test indentation of 20 vol% Al2O3/Mg disc. (b) High-magniﬁcation image of the area in the circle
in (a) (Al2O3particle size is 1mm).
0 6 10
10 20 30 0
Al2O3 particle size
Al2O3 Content (vol%)
Fig. 9 Relative Mg to MgO X-ray peak intensities for the Al2O3/Mg discs.
100 200 300 400
0 10 20 30
(testing powder) 0.3µm
Fig. 11 Eﬀect of Al2O3 content on the bending strength of Al2O3/Mg
not possible to directly compare these results with those obtained in the present study since the test pieces have diﬀerent shapes and diﬀerent bending test methods were used, these bending strengths are similar to those of the 0–20 vol% discs.
To enhance the mechanical properties of Mg alloys, over
10 vol% Al2O3/Mg powders were formed by ball milling
powder mixtures of pure Mg and Al2O3 particles with
particle sizes of 0.3 and 1mm. The eﬀect of the Al2O3content
of hot-pressed discs formed from the Al2O3/Mg powders on
the mechanical properties of the discs was investigated. The following results are obtained.
(1) For both Al2O3 particle sizes, the eﬀect of Al2O3
content on both the hardness and the bending strength of the Al2O3/Mg discs exhibited similar tendencies.
(2) The Al2O3/Mg discs containing 0.3mmAl2O3particles
had higher hardness and bending strength than those containing 1mmAl2O3 particles.
(3) The hardness of the Al2O3/Mg discs increased sharply
when the Al2O3 content increased from 10 to 20 vol%.
It subsequently decreased at 30 vol%.
(4) The reason for this sharp increase in hardness at an Al2O3content of 20 vol% is thought to be due to Al2O3
particle strengthening as a result of the excellent interfacial bonding between Mg and Al2O3 particles.
This will occur when the Al2O3/Mg discs contain
a suﬃcient amount of Al2O3 particles and have a
suﬃcient interparticle distance.
(5) The bending strength of the Al2O3/Mg plates increased
when the Al2O3 content was increased from 0 to
10 vol% and it subsequently decreased at 20 vol%.
(6) The 10 vol% Al2O3/Mg plates have a higher bending
strength than the 0 vol% plates. It is considered that both the 0 and 10 vol% plates have similar fracture
deﬂections and that the 10 vol% plates with Al2O3
particles can withstand higher compression and tension forces than the 0 vol% plates which do not contain any particles.
1) S. F. Hassan and M. Gupta: Mater. Sci. Eng. A392(2005) 163–168. 2) S. F. Hassan and M. Gupta: J. Metastable Nanocrystalline Mater.23
3) X. L. Zhong and M. Gupta: J. Metastable Nanocrystalline Mater.23
4) R. Unverricht, V. Peitz, W. Riehemann and H. Ferkel: Proc. Conf. on Magnesium Alloys and Their Applications, Deutsche, (Gesellschaft fur Materialkunde, 1998) pp. 327–332.
5) H. Oginuma and E. Yuasa: J. Jpn. Soc. Powder Powder Metall.52
6) H. Fujiwara, M. Nakatani, Y. Iwahashi and K. Ameyama: Adv. Mater.
7) S. Kawamori and T. Machida: Mater. Trans.48(2007) 373–379. 8) S. Housh,et al.:ASM Handbook Volume 2, (ASM international, 1990)
9) S. Ikeno, K. Matsuda, T. Matsuki, T. Suzuki, N. Endo, T. Kawabata and Y. Uetani: J. Mater. Sci.42(2007) 5680–5685.
10) M. M. Avedesian and H. Baker:ASM Specialty Handbook, Magnesium and Magnesium Alloys, (ASM international, 1999) p. 10.